Ferromagnetism induced by in-plane strain in a bulk VS2 based superlattice: (LiOH)0.1VS2
Sun, Ruijin; Deng, Jun; Ma, Yuxin; Hao, Munan; Chen, Xu; Meng, Dezhong; Zhao, Changchun; Du, Shixuan; Jin, Shifeng; Chen, Xiaolong; Chemical Communications  (2023) –; doi:10.1039/D3CC01662E

data_7131971
_publ_section_title
;
 Ferromagnetism induced by in-plane strain in a bulk VS2 based
 superlattice: (LiOH)0.1VS2
;
_journal_name_full               'Chemical Communications'
_journal_paper_doi               10.1039/D3CC01662E
_journal_year                    2023
_chemical_formula_moiety         'S10 V4.92, 0.42(O), 0.392(Li)'
_chemical_formula_sum            'Li0.39 O0.42 S10 V4.92'
_chemical_formula_weight         582.27
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_audit_update_record
;
2023-02-10 deposited with the CCDC.	2023-08-04 downloaded from the CCDC.
;
_cell_angle_alpha                78.327
_cell_angle_beta                 84.1363
_cell_angle_gamma                71.0231
_cell_formula_units_Z            1
_cell_length_a                   5.6557
_cell_length_b                   8.6279
_cell_length_c                   9.0552
_cell_measurement_reflns_used    4056
_cell_measurement_temperature    293
_cell_measurement_theta_max      31.03
_cell_measurement_theta_min      2.3
_cell_volume                     408.892
_diffrn_ambient_temperature      293
_diffrn_measured_fraction_theta_full 0.98
_diffrn_measured_fraction_theta_max 0.76
_diffrn_measurement_device       'Bruker D8 VENTURE PHOTO II'
_diffrn_measurement_device_type  'Bruker D8 VENTURE PHOTO II'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71075
_diffrn_reflns_av_R_equivalents  0.032
_diffrn_reflns_av_unetI/netI     0.0159
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            4056
_diffrn_reflns_theta_full        26.99
_diffrn_reflns_theta_max         31.03
_diffrn_reflns_theta_min         2.3
_exptl_absorpt_coefficient_mu    3.950
_exptl_absorpt_correction_T_max  0.7457
_exptl_absorpt_correction_T_min  0.1947
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_density_diffrn    2.339
_exptl_crystal_description       plate
_exptl_crystal_F_000             275
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_gt    5.4348
_refine_ls_goodness_of_fit_ref   1.1000
_refine_ls_number_constraints    0
_refine_ls_number_parameters     30
_refine_ls_number_reflns         1814
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.1320
_refine_ls_R_factor_gt           0.0671
_refine_ls_shift/su_max          0.0472
_refine_ls_shift/su_mean         0.0195
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     w=1/(\s^2^(I)+0.0004I^2^)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.1544
_refine_ls_wR_factor_ref         0.1715
_reflns_number_gt                246
_reflns_number_total             1814
_reflns_threshold_expression     I>3\s(I)
_cod_data_source_file            d3cc01662e2.cif
_cod_data_source_block           I
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_diffrn_radiation_probe' value 'X-ray' was changed to
'x-ray' in accordance with the
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

Automatic conversion script
Id: cif_fix_values 8170 2020-07-09 18:12:32Z antanas 
;
_cod_original_cell_volume        408.8919
_cod_database_code               7131971